**United States**
**Department of**
**Agriculture**
**Forest Service**
**Forest**
**Products**
**Laboratory**
**General**
**Technical**
**Report**
**FPL-GTR-76**

**Specific Gravity,**

**Moisture Content, and**

**Density Relationship**

**for Wood**

**Abstract**

**Contents**

This report reviews the basis for determining values for the density of wood as it depends on moisture content and specific gravity. The data are presented in several ways to meet the needs of a variety of users.

Keywords: Specific gravity, density, wood weight

*Page*

Introduction . . . 1

System for Determining Wood Density . . . 1

Density Tables . . . 2

Basic Specific Gravity . . . 2

Other Specific Gravity Values . . . 3

Concluding Remarks . . . 4

References . . . 4

Appendix. Relationship of Specific Gravity Values . . . 13

**July 1993**

**Simpson, William T. 1993. Specific gravity, moisture**
**content, and density relationship for wood. Gen. Tech.**
**Rep. FPL-GTR-76. Madison, WI: U.S. Department of**
**Agriculture, Forest Service, Forest Products Laboratory.**
**13 p.**

**A limited number of free copies of this publication**
**are available to the public from the Forest Products**
**Laboratory, One Gifford Pinchot Drive, Madison, WI**
**53705-2398. Laboratory publications are sent to more than**
**1,000 libraries in the United States and elsewhere.**

**The Forest Products Laboratory is maintained in **

United States
Department of
Agriculture
**Forest Service**
Forest
Products
Laboratory
General
Technical
Report
FPL-GTR-76

**Specific Gravity,**

**Moisture Content, and**

**Density Relationship**

**for Wood**

**William T. Simpson**

**Errata**

**Page 1, column 2, Equation (2)**

(2)
The term *Wd/V*g is related to basic specific gravity *G*b

by

**Pages 9-12, Tables 5-8. Note on tables should read**

Exceeds maximum possible moisture content

**Page 13, Appendix, Equation (la)**

(l*a)*
where Wd is oven-dry weight of wood, Vg is volume of
green wood, and pw is density of water.

**Page 13, Appendix, Equation (4**

**a)**

**a)**

**Specific Gravity, Moisture Content,**

**and Density Relationship for Wood**

**William T. Simpson, Research Forest Products Technologist**

**Forest Products Laboratory, Madison, Wisconsin**

**Introduction**

Knowledge about the density of wood is useful for
estimating shipping weights. The density of wood
depends on specific gravity and moisture content. A
common way to present density data is in tabular and
graphical form, where density in pounds per cubic foot
or kilograms per cubic meter is shown for a series of
specific gravity and moisture content values. This kind
of system is shown in the *Wood Handbook *(FPL 1987).
However, the system has several shortcomings.

One shortcoming is that density values in the *Wood*
*Handbook *are shown for moisture contents above the
maximum possible for those specific gravity values
(Tables 1 and 2). Another shortcoming is that this
system requires two steps: first, a graphical conversion
of specific gravity from one volume base to another,
and then a reading from a table. Furthermore, no
equations are offered for direct calculation of density
as a function of moisture content and specific gravity,
which precludes easy use of the system in computer
programs or spreadsheet calculations. Finally, the
system is subject to misinterpretation and thus can
yield erroneous density values if the user is not aware
of the various definitions of specific gravity as it applies
to wood.

This report discusses these shortcomings and develops equations, graphs, and tables for determining density as a function of moisture content and several common definitions of specific gravity.

**System for Determining**

**Wood Density**

The common definition of wood moisture content on a dry basis can be written as

(1)

where *W*g is the green weight of wood (pounds or

kilograms) at moisture content *M *(percent), and *W*d

is the oven-dry weight of wood.

Dividing both sides of Equation (1) by the volume of
wood at moisture content *M*(*V*g), the density *D *is

(2)

The term *W*d*V*g is related to basic specific gravity *G*b

by

(3)

where *p*w is the density of water (62.4 lb/ft3 or

1,000 kg/m3_{) based on volume when above 30 percent}

moisture content. Substituting Equation (3) into Equation (2) results in the following equation for calculating density:

(4)

A possible misapplication of Equation (4) is to use it
at <30 percent moisture content with no correction
in specific gravity for volumetric shrinkage. It is also
possible to overlook or misunderstand the definition of
specific gravity in the * Wood Handbook, *which could
cause a user to read incorrect density values from
the tables. Specific gravity is defined on the basis of
volume at the tabulated moisture content- not on
the more common basis of green volume, as is used
to define basic specific gravity. Misunderstandings
can cause errors 115 percent, as will be illustrated in
another section of this report.

The * Wood Handbook *describes a graphical way to
convert basic specific gravity to specific gravity based

**Figure 1—Relation of specific gravity to****moisture content. Follow line for specific gravity****(volume when green) to desired moisture****content, then read specific gravity (volume at****current moisture content) from vertical axis.****Source: Wood Handbook, Figures 3 and 4****(FPL 1987).**

on volume at any of the tabulated moisture contents (Fig. 1). Density values can then be read from the tables after the conversion. Although this system of determining density values is valid, it requires two steps and the use of both a graph and a table. The same density information can be presented in one table or one graph.

The maximum moisture content of wood is reached when the cell walls and cell lumens are completely filled with water. When specific gravity is high, lumen volume is low and maximum moisture content is

**2**

**Figure 2—Theoretical maximum possible****moisture content of wood (M****m a x*** ) as *a

**function****of basic specific gravity (G****b) .**

therefore restricted. This relationship can be estimated by

(5)

where *M*m a x is maximum moisture content and *G*w

is the specific gravity of wood substance, equal to approximately 1.54 (Skaar 1988). Equation (5) is shown in Figure 2.

Therefore, some density values at high specific gravity and moisture content values in Table 1 are not possible because the tabulated moisture content exceeds the maximum possible moisture content. These conditions will be discussed later in this report.

**Density Tables**

**Basic Specific Gravity**

Equation (4) can be used to change the basis of
tabulated density values below 30 percent moisture
content from specific gravity baaed on volume at
tabulated moisture content to basic specific gravity if
volume is corrected for shrinkage. Assuming a linear
relationship between shrinkage and moisture content
from 30 to 0 percent (Stamm 1964), the volumetric
shrinkage *S *at any moisture content is

(6)

where *a *is (30 - M)/30 and *S*t is total volumetric

Introducing Equation (6) into Equation (4) to account for shrinkage

(7)

Volumetric shrinkage data are necessary for using
Equation (7). Each species has its own *S*t value, and

ideally there would be a density table for each species. However, this would be somewhat cumbersome and may not be necessary, given the inherent variability of wood and the known relationship between volumetric shrinkage and basic specific gravity. Stamm (1964) summarized the background on this relationship. The result is that volumetric shrinkage of both hardwoods and softwoods can be reasonably approximated by

(8)

Therefore, even if a density table is not constructed for each species, Equation (8) accounts for the major source of variation in shrinkage between species.

Combining Equations (6) to (8) results in

(9)

The results of Equation (9) are listed in Table 3 and shown in Figure 3. Table 3 also shows maximum moisture content and density values. (The data in Table 3 are expressed in SI units in Table 4.)

The following example illustrates how using the
incorrect specific gravity results in an incorrect density
value. Suppose the user wants to know the density
of wood when specific gravity is 0.56 and moisture
content is 8 percent. If the volume basis for this given
specific gravity is not clear, or if the user is not aware
of the importance of the volume basis, the user might
go directly to the tabular data (Table 1) and read a
density of 37.7 lb/ft3 (605 kg/m3). If the given specific
gravity of 0.56 is the basic specific gravity, the correct
density is 42.3 lb/ft3_{ (679 kg/m}3_{) (Table 3) and the}

incorrect value is in error by 11 percent. Although this may seem an unlikely error for specialists in wood technology, it does not seem unlikely for someone who does not realize the necessity of knowing the exact definition of specific gravity for specific tables or handbooks. These definitions, if present, are often cited in footnotes that can be overlooked or ignored.

**Figure 3—Density of wood as a function of****moisture content and basic specific gravity (G****b****);**

**(a) English units, (b) SI units.**

**Other Specific Gravity Values**

Some references list specific gravity values on a basis other than green volume; in those cases, Table 3 is of no use in determining density values. Oven-dry volume (Hildebrand 1970) and volume at 12 percent moisture content (Chichignoud and others 1990) are common alternative bases. Equation (9) can be generalized for specific gravity baaed on volume at any moisture content if we develop the relationship between basic specific gravity and specific gravity based on the other volumes (Appendix). The result of this relationship is

(10)

where *GM* is specific gravity based on volume at

moisture content *M. *Equation (10) is substituted
into Equation (9) for moisture contents <30 percent
and into Equations (3) and (4) for moisture contents
>30 percent.

Table 5 is a density table for specific gravity based on
volume at 12 percent moisture content *(GM*= *G*1 2)

(see Table 6 for SI units). Table 7 shows specific
gravity values based on oven-dry volume *(GM* = *G*O)

(see Table 8 for SI values).

**Concluding Remarks**

The validity and efficiency of a method for determining the density of wood at various combinations of

specific gravity and moisture content depend on an understanding of the definition of specific gravity. Because specific gravity depends on wood volume, shrinkage must be accounted for when determining specific gravity below the fiber saturation point. The equations and tables described in this report can be used to determine density at any moisture content and specific gravity.

**References**

**Chichiguoud, M.; Deon, G.; Detienne, P.; Parant, B.;**
**and Vantomme, P. **1990. Tropical timber atlas of Latin
America. Yokohama, Japan: International Tropical
Timber Organization, and Nogent-Sur-Marne Cedex,
France: Centre Technique Forestier Tropical.

**Forest Products Laboratory. **1987. Wood handbook:
Wood as an engineering material. Agric. Handb.
72. (Rev.) Washington, DC: U.S. Department of
Agriculture. 466 p.

**Hildebrand, R. **1970. Kiln drying of sawn timber.
Germany: Maschinenbau GmbH. 198 p.

**Skaar, C. **1988. Wood-water relations. New York:
Springer-Verlag. 283 p.

**Stamm, A.J. **1964. Wood and cellulose science.
New York: The Ronald Press. 549 p.

**Appendix. Relationship of**

**Specific Gravity Values**

In this appendix, we describe the general relationship between basic specific gravity and specific gravity values baaed on volume at other moisture content levels.

The next step is to express *S*t in Equation (6a)

in terms of *GM. *Substituting Equation (6a) into

Equation (8) *(S*t = 0.265 *G*b*) *in the text

Basic specific gravity is defined as

**(1****a****)**

where *W*d is oven-dry weight of wood, *V*d is volume of

dry wood, and *p*_{w}is density of water.

Specific gravity baaed on volume at any other moisture
content *M *is defined as

Solving for *S*t

(8*a*)

and substituting Equation (8a) into Equation (6a)

Equating Equations (1a) and (2a) through *W*d

(2*a*)

(3*a*)

where *V*gis volume of green wood.

Volumetric shrinkage S from >30 percent to <30 per-cent moisture content is

which can be substituted into Equation (9) in the text to calculate density based on the volume at any moisture content. Equation (9a) can also be used to calculate the graphical relationship between moisture content, basic specific gravity, and specific gravity based on volume at any moisture content, as shown in Figure 1 of the text.

or

Substituting Equation (4a) into Equation (3a)

(4*a*)

(5*a*)

Assuming the linear shrinkage of Equation (6) in the
text (*S *= *aS*t)

The value of *M *in the term a ((30 - *M)/30) *in
Equation (9a) is the moisture content for the volume
base of the specific gravity. The value of *M *in the
term * a *in Equation (9) in the text is the moisture
content at which the density is calculated (that is, 0
to 200 percent in Tables 5 and 7). If this latter value
of

*M*is taken as the moisture content of the specific gravity volume base, the resulting density values will be baaed on the specific gravity at the volume of the tabulated moisture content, that is, the same as that in the tables in the

*Wood Handbook.*Note also in Equation (9a) that when

*M*= 30,

*a*= 0, and

*GM*=

*G*b, text Equation (9) reverts to text Equations (3)

and (4).
where a is (30 - M)/30.
(6*a*)
(7*a*)
(9* _{a}*)
13